Simultaneous determination of several crystal structures from powder mixtures: the combination of powder X-ray diffraction, band-target entropy minimization and Rietveld methods
Schreyer, Martin; Guo, Liangfeng; Thirunahari, Satyanarayana; Gao, Feng; Garland, Marc; Journal of Applied Crystallography 47 (2014) 659–667; doi:10.1107/S1600576714003379

data_2300448
_publ_section_title
;
 Simultaneous determination of several crystal structures from powder
 mixtures: the combination of powder X-ray diffraction, band-target
 entropy minimization and Rietveld methods
;
_journal_coeditor_code           to5064
_journal_issue                   2
_journal_name_full               'Journal of Applied Crystallography'
_journal_page_first              659
_journal_page_last               667
_journal_paper_doi               10.1107/S1600576714003379
_journal_volume                  47
_journal_year                    2014
_chemical_formula_analytical     'Al2 O3'
_chemical_formula_iupac          'Al2 O3'
_chemical_formula_moiety         'Al2 O3'
_chemical_formula_structural     'Al2 O3'
_chemical_formula_sum            'Al2 O3'
_chemical_formula_weight         101.96
_chemical_name_mineral           corundum
_chemical_name_systematic        'aluminium oxide'
_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.758152(42)
_cell_length_b                   4.758152(42)
_cell_length_c                   12.98970(18)
_cell_measurement_temperature    298
_cell_volume                     254.687(5)
_computing_cell_refinement       'Topas v4.2 (Bruker AXS GmbH, 2009)'
_computing_data_collection       unknown
_computing_data_reduction        'Topas v4.2 (Bruker AXS GmbH, 2009)'
_computing_molecular_graphics    'Diamond 3.1f'
_computing_publication_material  CSD
_computing_structure_refinement  'Topas v4.2 (Bruker AXS GmbH, 2009)'
_computing_structure_solution    'Topas v4.2 (Bruker AXS GmbH, 2009)'
_diffrn_ambient_temperature      298
_diffrn_detector                 'Proportional Counter'
_diffrn_detector_type            'gas filled point detector'
_diffrn_measurement_device_type  'Philips 3020'
_diffrn_radiation_monochromator  'Diffracted beam Graphite'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_wavelength     1.54180
_diffrn_source                   'sealed X-ray tube'
_diffrn_source_target            Cu
_exptl_absorpt_coefficient_mu    12.608
_exptl_crystal_density_diffrn    3.989
_exptl_crystal_F_000             300
_pd_block_diffractogram_id       al2o3_profile
_pd_char_colour                  colourless
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        150
_pd_meas_2theta_range_min        5
_pd_meas_number_of_points        7250
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.02
_pd_proc_2theta_range_max        150
_pd_proc_2theta_range_min        5
_pd_proc_info_excluded_regions   0
_pd_proc_ls_background_function  'Chebychev of order 3, plus 1/x'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     'fundamental parameter'
_pd_proc_ls_prof_R_factor        0.118
_pd_proc_ls_prof_wR_expected     0.247
_pd_proc_ls_prof_wR_factor       0.236
_refine_ls_goodness_of_fit_all   0.095
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           fullcycle
_refine_ls_number_constraints    0
_refine_ls_number_parameters     12
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            0.018
_refine_ls_shift/su_max          .01
_refine_ls_structure_factor_coef Inet
_refine_ls_weighting_details     1/[Y~i~+\s(Y~i~)]
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            to5064sup1.cif
_cod_data_source_block           Al2O3_BTEM
_cod_original_cell_volume        254.6868(58)
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_database_code               2300448
_cod_database_fobs_code          2300448